Logic Gates

Thermal AND Gate Using a Monolayer Graphene Nanoribbon Souvik Pal and Ishwar K. Puri*

The

first ever implementation of a thermal AND gate, which performs logic calculations with phonons, is presented using two identical thermal diodes composed of asymmetric graphene nanoribbons (GNRs). Employing molecular dynamics simulations, the characteristics of this AND gate are investigated and compared with those for an electrical AND gate. The thermal gate mechanism originates through thermal rectification due to asymmetric phonon boundary scattering in the two diodes, which is only effective at the nanoscale and at the temperatures much below the room temperature. Due to the high phonon velocity in graphene, the gate has a fast switching time of ≈100 ps.

1. Introduction Logic calculations performed with phonons are referred to as phononics.[1] The functional building block of phononic devices is the thermal diode. It allows heat to flow in a single direction and prevents its flow in the opposing direction.[2–4] Experimental,[5] theoretical[6,7], and molecular simulation[8–12] investigations have proposed different material systems for thermal diodes, e.g., mass graded CNT,[13] the polyethylene-silicon interface,[9] carbon nanocone,[10] graphene nanoribbon (GNR),[8] and solid-fluid interfaces.[2,3] However, more complex structures such as thermal logic gates, thermal memory[14] and thermal transistors[4,15,16] that combine thermal diodes have been sparingly investigated. In most materials, thermal rectification depends on phonon transport at the nanoscale. At this scale, interfaces and boundaries scatter phonons and impede thermal transport.[17] Hence, the design of phononic circuits to S. Pal, Prof. I. K. Puri Department of Mechanical Engineering McMaster University Hamilton ON L8S 4L7, Canada E-mail: [email protected] Prof. I. K. Puri Department of Engineering Physics McMaster University Hamilton ON L8S 4L7, Canada DOI: 10.1002/smll.201303888 small 2015, DOI: 10.1002/smll.201303888

produce prescribed interfacial and boundary scattering is a challenging task. Prior investigations of thermal logic gates[18] have been based on ideal nonlinear atomic chain segments which do not exactly correspond to a real material. For any logic device, the “HIGH”, i.e., digital logic 1 and “LOW”, or digital logic 0 states must be established. For a typical electrical diode, a voltage range determines these states. Since the analog of voltage for a thermal logic device is temperature, the “LOW” and “HIGH” states of a thermal device are similarly prescribed by a temperature range. We present the first design of a thermal AND gate using a GNR thermal diode as its fundamental building block. The asymmetric shape of the GNR diode produces asymmetric phonon boundary scattering. Thus, the diode exhibits high rectification, described as the ratio of forward to reverse current. Using molecular dynamics (MD) simulations, we characterize the performance of the thermal AND gate by investigating the fundamental behavior of the gate, identifying optimal operating conditions, and characterizing its switching behavior.

2. Results and Discussion The basic design of a typical GNR diode is shown in Figure 1(a) where higher heat current flows from the wider to the narrower terminal, i.e., J+ > J–. In Figure 1(b) a typical electrical AND gate implemented by two diodes D1 and D2 is shown. It has two input terminals, an output terminal and a biasing terminal. The device has predefined “HIGH” and © 2015 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim

www.small-journal.com

1

full papers www.MaterialsViews.com

“LOW” voltage ranges. The output voltage is “HIGH” when both the inputs are “HIGH”. The biasing terminal, usually maintained at “HIGH”, is connected to the output terminal through a biasing resistance. Figure 1(c) presents the thermal analog of the electrical AND gate of Figure 1(b). It is implemented through the two GNR diodes shown in red and blue and the biasing terminal represented by green. The two diodes are connected to the biasing terminal through a very narrow region shown in purple that offers high thermal resistance due to strong boundary phonon scattering. The entire system consists of 15372 C atoms. For the base case, we assume 300 K to be “HIGH” and 100 K as “LOW” for the system. The biasing terminal is also maintained at “HIGH”. The temperatures at input 1, input 2, biasing and output terminals are designated as T1, T2, Tb, and To, respectively. Four different T1–T2 combinations are simulated, viz., 0–1, 1–0, 1–1 and 0–0. For the 1–0 case, i.e., when T1 = 300 K, T2 = 100 K, diode 2 is forward biased and diode 1 is reverse biased. For this case, the y-averaged temperature distribution along x in the two diodes is shown in Figure 2(a) and 2(b). For both diodes, the temperature remains almost constant within the x bounds of the output region (illustrated by dotted lines). The x-averaged temperature distribution along y in the shaded region including the output is shown in Figure 2(c). Again, within the y bounds of the output region, the temperature does not change appreciably. The steady state average output temperature To = 155 K with any spatial or temporal fluctuations lying within 1%. The

temperature distribution in the biasing terminal and the resistance is shown in Figure 2(d). The large drop across the narrowest section of the resistance is due to strong boundary phonon scattering. In an ideal AND gate, when either of the inputs is low, the expected output is “LOW”. To represent the effectiveness of the AND gate, we define an output parameter

ε = ( Output − LOW ) / ( HIGH − LOW ) .

(1)

An ideal AND gate should demonstrate ε = 0 for 0–1, 1–0 and 0–0 inputs. The inputs and their corresponding outputs in terms of ε for the simulated base case thermal AND gate are presented as the truth table in Table 1. In classical MD simulations, the temperature, TMD =

pi2 2 . ∑ 3Nk b i 2 mi

(2)

Here, TMD represents temperature calculated through the MD simulation, N the total number of atoms considered, kb the Boltzmann constant, and pi and mi the momentum and mass of ith atom. When the system temperature is lower than the Debye temperature of the material, quantum effects on thermal transport can no longer be neglected.[19] By equating the total energies obtained from the quantum and classical representation of the system, we relate the two temperatures TMD and TQ,[20]

Figure 1. a) A single GNR diode is shown with heat currents J+ and J–. Here, J+ > J–, which indicates that the GNR diode prefers heat current to flow from the wider to the narrower terminal. b) A typical electrical AND gate implemented by two electrical diodes is shown. It has two input terminals, an output and a biasing terminal, which is connected to the output terminal via a biasing resistance. c) The thermal AND gate analogous to the electrical AND gate of Figure 1(b) is presented. The gate consists of two GNR diodes shown in red and blue and is identical to the one shown in Figure 1(a). These two diodes are connected to a biasing terminal via a converging–diverging region of very narrow section serving as biasing resistance. Similar to the electrical diode, it also contains two input terminals, an output terminal and a biasing terminal. The edge atoms of the inputs and the biasing terminal are held fixed. The next eight layers of atoms are bath atoms shown in deeper shades of red, blue, and green. The entire diode consists of 15372 atoms.

2 www.small-journal.com

© 2015 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim

small 2015, DOI: 10.1002/smll.201303888

www.MaterialsViews.com

Figure 2. a) The y-averaged temperature distribution along x at steady state in diode 2 is shown. The input 2 terminal is maintained at “LOW”, i.e., 100 K. The temperature does not change appreciably within the x bounds of the output region, i.e., ±5 Å. b) The y-averaged temperature distribution along x at steady state for diode 1 is shown. The input 1 terminal is held at “HIGH”, i.e., 300 K. Again, the temperature changes very little within the x bounds of the output region. c) The x-averaged temperature distribution along y at steady state is plotted in the shaded region which extends from –5 to 5 Å along x. d) the y-averaged temperature distribution along x in the biasing terminal and the resistance is shown. For all temperature plots, error bars are not shown for the sake of presentation clarity. The variations of temperature at steady state are within 1% of their average value.

TMD =

2TQ3 TD /TQ x 2 dx, TD2 ∫0 e x − 1

(3)

where TD represents the Debye temperature and TQ the quantum corrected temperature. Since the reported range of Debye temperature for graphene varies, from between 1000–2300 K[21–23] to 322 K,[24–26] the benefit of employing this correction is ambiguous. We assume the Debye temperature to be 322 K since this temperature has been used for quantum corrections for thermal rectification studies in single layer GNRs.[25,26] The value of ε for a 1–0 input increases slightly from 0.275 to 0.28 as a result of the correction. This small ≈2% change suggests a weak influence of the

Table 1. The truth table. Input 2

Output [ε]

Ideal

1

0

0.270

0

0

1

0.275

0

0

0

0.025

0

1

1

0.993

1

Input 1

small 2015, DOI: 10.1002/smll.201303888

quantum correction. Hence, for the following discussion, we will neglect its influence. In a practical implementation of an electrical AND gate, when either of the inputs is “LOW”, the output voltage is higher than “LOW” due to a small voltage drop VD in a forward biased diode. For instance, a typical silicon diode in forward bias has VD = 0.6 V.[27] With 5 V as “HIGH” and 0 V as “LOW”,[28] the output of the AND gate shown in Figure 1(b) is 0.6 V, or ε = 0.12. Thus, the output is designated as “LOW” if 0 ≤ ε ≤ 0.12. For the thermal AND gate output shown in Table 1, this range is 0 ≤ ε ≤ 0.275, or 100 K ≤ To ≤ 155 K . From Figure 2(b), the forward bias temperature drop ΔD across diode 2 is 55 K, which is much lower than the 145 K drop across diode 1 that is reverse biased. Similarly, the output is designated “HIGH” if 0.99 ≤ ε ≤ 1. An effective AND gate must have very narrow ranges for “HIGH” and “LOW”. We define the upper limit of the “LOW” range as ε , i.e., 0 ≤ ε ≤ ε where ε corresponds to the output ε for the 1–0 or 0–1 cases. The output ε for the 0–0 case lies between 0 and ε . For the current AND gate, ε = 0.275. The smaller the value of ε the better is the gate. The least effective AND gate will have 0 ≤ ε ≤ 0.5 and 0.5 ≤ ε ≤ 1 as “LOW” and “HIGH” ranges. If ε > 0.5, the device no longer operates as an AND gate.

© 2015 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim

www.small-journal.com

3

full papers www.MaterialsViews.com

Figure 3. The heat currents flowing in the gate at steady state are shown. The heat current Ji2 into the diode 2 equals the sum of heat currents Ji1 from the diode 1 and Jb from the biasing terminal.

Figure 3 shows the heat current in the gate at steady state. The total current Ji2 flowing into input 2 equals the sum of the currents Ji1 from input 1 and Jb from the biasing terminal, thereby satisfying energy conservation. Ji1 = 0.9Ji2 is a leakage current flowing from the “HIGH” to “LOW” terminals. This is different from an electrical AND gate where there is no leakage current flowing from the “HIGH” to “LOW” terminals. A thermal diode has a relatively smaller reverse bias resistance as compared to an electrical diode. The much higher reverse bias resistance in a typical electrical diode leads to a rectification ratio J + / J − , i.e., a forward to reverse bias current ratio of about 1000.[29] The highest rectification ratio reported for a thermal diode is 4.5.[8] With the GNR diode of Figure 1(a) it is 1.94. This low rectification ratio leads to a significant leakage current from the “HIGH” to “LOW” terminals. (Details of obtaining J + / J − for the single GNR diode of Figure 1(a) are available in the supporting information.) To understand why the temperature drop across diode 2 is smaller than for diode 1, we compare the phonon power spectrum for atoms contained in different sections of the two diodes. An overlap in the phonon spectrum over different portions of a material facilitates phonon motion without scattering while a mismatch in the spectra produces scattering which lowers the phonon thermal conductivity and impedes phonon transport.[30] The spectrum P(f) is determined by taking the Fourier transform of the velocity autocorrelation function obtained from the MD trajectories.[9,31] For each diode, we calculate two spectra, one for the layer of atoms adjacent to the heat bath (layer C for diode 1 and layer B for diode 2) and another for the layer of atoms at x = 0 (layer D for diode 1 and layer A for diode 2), as shown in Figure 4(a) and (b). Clearly, there is significantly higher spectral overlap between layers A and B as compared to that between layers C and D. The direction of heat transfer in diode 1 is from layer C to layer D while that in diode 2 is from layer A to

4 www.small-journal.com

Figure 4. a) The steady state phonon spectrum for atoms in layers A and B in diode 2 is presented. Layer B is immediately next to the heat bath. Layer A lies at the center of the x bounds of the output region, i.e., at x = 0. b) The steady state phonon spectrum for atoms in layer C and D in diode 1 is presented. Layer C is adjacent to the heat bath. Layer D lies at x = 0.

layer B. Thus, for a GNR diode, the spectral overlap increases when heat transfer occurs from the wider to the narrower terminal, as in diode 1, favoring greater thermal transport in contrast to thermal transport the opposite direction, i.e., from narrower to the wider terminal in diode 2. In asymmetric GNR thermal diodes, this spectrum modification is produced by the asymmetric boundary scattering of phonons at different locations.[8] The higher impedance to phonon transport from layer C to D makes diode 1 to become reverse biased and thereby induces a relatively larger temperature drop of T1–To = 145 K as compared to a smaller drop of To–T2 = 55 K across the forward biased diode 2. It is worth noting that in Figure 2(b), the temperature drop in diode 1 is highly nonlinear in the vicinity of the heat bath. This is attributed to the much localized spectral mismatch in diode 1 that produces impedance to phonon transport. To prove this, we establish a quantitative measure of the spectral mismatch between two spectra P1(f) and P2(f) as,

© 2015 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim

small 2015, DOI: 10.1002/smll.201303888

www.MaterialsViews.com

output temperature? At room temperature, graphene has a phonon mean free path (mfp) of ≈775 nm,[32] which is much larger than the length scale L for the base case AND gate. Consequently, thermal transport is significantly influenced through phonon boundary scattering, which primarily controls thermal rectification in the diodes. The influence of boundary scattering could be eliminated by simulating the AND gate at a length significantly larger than 775 nm. However, such a system would require enormous computational resources. At the larger length scale, phonon transport is diffusive, allowing us to model the heat transfer through the continuum 2D diffusion equation, which at steady state is, ∂2T ∂2T + = 0. ∂x 2 ∂ y2

Figure 5. a) An expanded image of diode 1 is shown where seven layers of atoms, numbered 1–7, are highlighted in deep pink along with the layer C that is immediately next to the heat bath and shown in black. For each of the seven layers, the spectral overlap parameter S is calculated between that layer and layer C. b) The resulting values of S for each of the seven layers with respect to their x-position are plotted. ∞

S=

∫

P1 ( f ) P2 ( f ) df

0

⎛∞ ⎞ ⎛∞ ⎞ P f df ( ) 1 ⎜∫ ⎟ ⎜ ∫ P2 ( f ) df ⎟ ⎝0 ⎠⎝0 ⎠

.

(4)

S = 1 and S = 0 correspond to the complete spectral overlap and complete spectral mismatch conditions, respectively. We calculate S between layer C and each of the seven other layers shown in Figure 5(a). A plot of S with respect to the position of those layers along x is presented in Figure 5(b). This exercise helps us understand how the phonon spectrum changes along the direction of heat transfer in diode 1. For layer 1, S ≈ 1, indicating almost complete overlap with the layer C spectrum. However, for layers 2–4, the overlap with the layer C spectrum, indicated by decreasing S, drops significantly over a very small distance but shows little change beyond layer 5. The steep change in the phonon spectrum from layer C to layer 4 causes significant phonon scattering, The bulk of the temperature drop occurs in this region. However, after this section the phonon spectrum does not change appreciably. This implies that beyond layer 5 there are high spectral overlaps between layers, i.e., very little phonon scattering occurs beyond layer 5. Hence, the temperature drop is very small in this region. The change in the phonon spectrum is highly nonuniform and also very localized. This leads to localized increase in the impedance to phonon transport and explains the strong nonlinearity of the temperature profile close to the heat bath in diode 1. It is worth asking, if there were no rectification at all from the individual GNR diodes, what would have been the small 2015, DOI: 10.1002/smll.201303888

(5)

The steady state temperature obtained by solving Equation (5) for an equivalent continuum system is shown in Figure 6. The continuum system is isometrically scaled up with the ratios of the lengths of different sections held unaltered. The temperature distribution shown in Figure 6 is independent of the thermal conductivity and length scale L, as long as L mfp of phonons, since at this scale, boundary scattering has a weak influence on thermal transport as compared to Umklapp phonon-phonon scattering. The independence of the steady state temperature contours with respect to the thermal conductivity κ are apparent because κ is absent from Equation (5). The spatiotemporal averaged temperature at the output section is 220 K which is significantly higher than the temperature obtained with the smaller graphene AND gate. The corresponding value of ε is 0.6, which is outside the maximum allowed range 0 ≤ ε ≤ 0.5 for the output to be designated as “LOW”. Hence, the continuum system does not behave as an AND gate. This establishes that thermal rectification is essential in obtaining AND gate behavior, which is achieved at very small length scales due to the strong boundary scattering of phonons.

Figure 6. Steady state temperature contours in a 2D region that is similar in shape to the thermal AND gate in Figure 1(c) but with L = 251 mm is shown. The edges at the input and biasing terminals are subjected to Dirichlet boundary conditions while all other edges are subjected to adiabatic boundary condition.

© 2015 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim

www.small-journal.com

5

full papers www.MaterialsViews.com

Figure 7. The variation of ε for 1–0 input with variations in values for “HIGH” and “LOW” are shown. Three values of “HIGH” = 300 K, 400 K, and 500 K are used. For each of these, five simulations are run with five different “LOW” values such that Δ varies from 40 to 200 K in steps of 40 K, where Δ = ′HIGH′ − ′LOW′ . The three sets with different “HIGH” values’ are represented with different symbols.

Figure 8. Switching characteristic of the AND gate is shown. At steady state for the base case with 1–0, the input 2 is switch to logic 1. The transient evolution of ε is plotted over time. The error bar representing the error in ε calculated over the temperature of all atoms in the output region. In this figure, t = 0 represents steady state. After 80 ps the input is switched.

We now investigate the ranges of operating temperature that lead to the most effective operation of the AND gate, i.e., the smallest possible value of ε . For this, we compare ε obtained for the 1–0 input cases with different “HIGH” and “LOW” temperatures. Simulations are run for three different “HIGH” temperatures of 300 K, 400 K and 500 K. For each such value, five simulations are run with different “LOW” values such that ΔT = “HIGH”—“LOW”, varies from 40 to 200 K. The resulting plot of ε vs. ΔT is presented in Figure 7. The base case corresponds to ΔT = 200 K when “HIGH” is 300 K. For all three “HIGH” temperatures, when Δ ≤ 80 K the device performance is very poor because ε is close to 0.5. Increasing Δ beyond 80 K improves device performance, as indicated by the decrease in ε when “HIGH” = 300 K. Very little additional improvement in ε occurs for the other two cases when “HIGH” = 400 K or 500 K. This reveals the decreasing efficacy of thermal rectification with increasing temperature. The rectification mechanism based on phonon boundary scattering that limits thermal conductivity and phonon transport is more apparent at low temperatures. At temperatures higher than 80 K, the effect of Umklapp phonon-phonon scattering on heat transfer starts to become comparable to that of boundary scattering.[33] At room temperature, Umklapp phonon-phonon scattering dominates over boundary scattering.[34] When “HIGH” = 300 K and “LOW” = 100 K, most regions of the device are at temperatures significantly lower than 300 K, as is evident from Figure 2, i.e., boundary scattering is still effective. Increasing “LOW” from 100 K, i.e., decreasing Δ from 200 K, this effectiveness diminishes, leading to a deterioration in performance. With “HIGH” = 400 K or 500 K, Umklapp phonon scattering eliminates the influence of boundary scattering and the device performance is even worse. Finally, we characterize the response of the AND gate to a rapidly changing input. In a practical implementation,

an AND gate is subjected to continuously changing streams of 1 and 0 states at the two inputs. The pace at which the output can keep abreast of changes in the input is called the switching time, which is an important property of a diode. To examine the thermal switching time, we first obtain a steady state for the base case with the 1–0 state and then abruptly change the temperature at the “LOW” terminal to “HIGH”, i.e., to 300 K, thereby changing to a 1 – 1 condition. The resulting alteration in the output ε with respect to time is presented in Figure 8, where t = 0 corresponds to steady state and the input 2 is switched at t = 80 ps. The device output ε responds to this change by attaining a value close to 1 in about 100 ps, which represents the switching time. This time is comparable to that for a fast response electrical diode, such as the Schottky diode which has a switching time between 10 to 100 ps.[35] The fast response of the thermal device can be attributed to the very high phonon speed in grapheme, which is ≈2 × 104 m s−1.[36]

6 www.small-journal.com

3. Conclusion In summary, A thermal AND gate is implemented using GNR diodes and represents the first study of such a gate using existing nanomaterials. Employing molecular dynamics simulations, the diode performance is characterized. The output from the diode is presented in the form of a truth table. The range of output temperatures that can be designated as “HIGH” and “LOW” are identified. With either inputs at a logic 0 state, the device output parameter ε is in the range 0 ≤ ε ≤ 0.275 , which is comparable to that for a typical silicon based electrical diode (0 ≤ ε ≤ 0.12 ). The working mechanism of the thermal AND gate is controlled by the thermal rectification effect in the two diodes. This rectification occurs due to asymmetric phonon boundary scattering, which is significant at the nanoscale when the device length

© 2015 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim

small 2015, DOI: 10.1002/smll.201303888

www.MaterialsViews.com

is comparable to the phonon mfp. Thus, such a device loses its efficacy at continuum length scales. The device performs better at temperatures lower than 300 K when boundary scattering dominates over phonon-phonon Umklapp scattering. The switching speed of the AND gate is ≈100 ps, which is comparable to that for fast electrical diodes. This is attributed to the fast phonon propagation speed of 2 × 104 m s−1 in graphene. The results imply there is significant potential to implement GNR diodes in phononic logic circuits and thus perform computations with phonons.

4. Experimental Section Molecular simulations have described thermal transport in a monolayer graphene sheet and GNRs.[37–41] Typically, in such simulations, the atoms at the two edges of the graphene sheet are held fixed. The next few atomic layers at both ends are used as the heat source and sink to initiate heat transfer with a nonequilibrium molecular dynamics (NEMD) simulation. We also adopt this standard methodology. The edge atoms of the input and biasing terminals in Figure 1(c), shown in black, are held fixed. The next eight atomic layers, shown in deeper shades of red, green, and blue are used as heat baths that are maintained at fixed temperatures by a Nosé–Hoover thermostat, which is used to initiate heat transfer in GNR investigations.[20,25,41] Results of MD-based studies of thermal transport in nanostructures can be sensitive to the size of the heat bath due to the presence of a localized edge mode (LEM) of phonons that lie close to the boundaries.[42] We use eight layers of heat bath atoms, which are sufficient for removing this LEM effect on thermal transport.[41,42] At steady state, the device output is recorded as the average temperature in the 1 × 1 nm square region centered on the origin. All structures are generated using VMD[43] and Xenoview.[44] The interatomic interactions between carbon atoms in graphene are described by the second generation reactive bond order potential (REBO II),[45] which accurately reproduces graphene properties, particularly bond strength and anharmonicity.[46] We apply nonperiodic boundary conditions in all directions and a timestep of 1 femtosecond (fs). All simulations are performed using LAMMPS.[47] The system energy is first minimized using the conjugate gradient technique.[47] The minimized structure is then initialized at 300 K. Next, the system is equilibrated under canonical (NVT) ensemble at T = 300 K for 0.2 nanoseconds (ns) with the temperature being controlled by Nosé–Hoover thermostat that has a coupling time of 1 picosecond (ps). Finally, the system is equilibrated under an NVE ensemble for 0.2 ns. After equilibration, heat transfer is initiated by Nosé–Hoover thermostats that have the same coupling time of 1 ps for the heat bath atoms at the inputs and the biasing terminal. The heat currents Ji1, Ji2, and Jb associated with the thermostats at input 1, input 2 and the biasing terminal are calculated from the rate of energy added or subtracted to each thermostat. At steady state, which is generally achieved after 2 × 106 steps, i.e., 2 ns, the heat currents become steady, fluctuating only within ≈3% of their average values. The method to calculate J from the simulation data is described in the supporting information.

small 2015, DOI: 10.1002/smll.201303888

Supporting Information Supporting Information is available from Wiley Online Library or from the author.

Acknowledgements This research was supported by a grant from the National Science Foundation (CBET 1246611). We thank the Virginia Tech Department of Engineering Science and Mechanics for the use of its Linux Computing Cluster.

[1] [2] [3] [4] [5] [6] [7] [8] [9] [10] [11] [12] [13] [14] [15] [16] [17]

[18] [19] [20] [21] [22] [23] [24] [25] [26] [27] [28] [29] [30] [31] [32]

[33]

L. Wang, B. Li, Phys. World 2008, 21 (3), 27. S. Murad, I. K. Puri, J. Chem. Phys 2012, 137 (8), 081101. S. Murad, I. K. Puri, Appl. Phys. Lett. 2012, 100 (12), 121901. S. Murad, I. K. Puri, Appl. Phys. Lett. 2013, 102 (19), 193109. C. W. Chang, D. Okawa, A. Majumdar, A. Zettl, Science 2006, 314 (5802), 1121. N. Zeng, J.-S. Wang, Phys. Rev. B 2008, 78 (2), 024305. E. Pereira, Phys. Lett. A 2010, 374 (19), 1933. N. Yang, G. Zhang, B. Li, Appl. Phys. Lett. 2009, 95 (3), 033107. M. Hu, P. Keblinski, B. Li, Appl. Phys. Lett. 2008, 92 (21), 211908. N. Yang, G. Zhang, B. Li, Appl. Phys. Lett. 2008, 93 (24), 243111. M. Hu, J. V. Goicochea, B. Michel, D. Poulikakos, Appl. Phys. Lett. 2009, 95 (15), 151903. M. Alaghemandi, F. Leroy, F. Müller-Plathe, M. C. Böhm, Phys. Rev. B 2010, 81 (12), 125410. M. Alaghemandi, F. Leroy, E. Algaer, M. C. Böhm, F. Müller-Plathe, Nanotechnology 2010, 21 (7), 075704. L. Wang, B. Li, Phys. Rev. Lett. 2008, 101 (26), 267203. B. Li, L. Wang, G. Casati, Phys. Rev. Lett. 2004, 93 (18), 184301. S. Murad, I. K. Puri, J. Chem. Phys 2013, 139 (15), 151102. G. Balasubramanian, S. Banerjee, I. K. Puri, Interfacial Thermal Resistance in Nanoscale Heat Transfer. In IMECE 2008, ASME: Boston, Massachusetts, USA, 2008; Vol. 10, pp 969. L. Wang, B. Li, Phys. Rev. Lett. 2007, 99 (17), 177208. J. Chen, G. Zhang, B. Li, Appl. Phys. Lett. 2009, 95 (7), 073117. J. Hu, X. Ruan, Z. Jiang, Y. P. Chen, AIP Conf. Proc. 2009, 1173 (1), 135. V. K. Tewary, B. Yang, Phys. Rev. B 2009, 79 (12), 125416. T. Tohei, A. Kuwabara, F. Oba, I. Tanaka, Phys. Rev. B 2006, 73 (6), 064304. X. Zhai, G. Jin, EPL (Europhys. Lett.) 2011, 96 (1), 16002. J. Hu, X. Ruan, Y. P. Chen, Nano Lett. 2009, 9 (7), 2730. C. Yu, G. Zhang, J. Appl. Phys. 2013, 113 (4), 044306. X. Li, P. Yang, Int. J. Mater. Struct. Integrity 2013, 7 (1), 131. P. Bajec, B. Pevec, D. Voncina, D. Miljavec, J. Nastran, IEEE T. Ind. Electron. 2005, 52 (2), 436. I. L. Sziebert, Motor control circuit and method with digital level shifting. US 6064174 A, 2000. R. Ajimsha, M. Jayaraj, L. Kukreja, J. Electron. Mater. 2008, 37 (5), 770. N. Li, J. Ren, L. Wang, G. Zhang, P. Hänggi, B. Li, Rev. Mod. Phys. 2012, 84 (3), 1045. R. Bhowmik, K. S. Katti, D. Katti, Polymer 2007, 48 (2), 664. S. Ghosh, I. Calizo, D. Teweldebrhan, E. P. Pokatilov, D. L. Nika, A. A. Balandin, W. Bao, F. Miao, C. N. Lau, Appl. Phys. Lett. 2008, 92 (15), 151911. D. L. Nika, E. P. Pokatilov, A. S. Askerov, A. A. Balandin, Phys. Rev. B 2009, 79 (15), 155413.

© 2015 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim

www.small-journal.com

7

full papers www.MaterialsViews.com [34] W. J. Evans, L. Hu, P. Keblinski, Appl. Phys. Lett. 2010, 96 (20), 203112. [35] A. Grndl, B. Hoffmann. Half-bridge subassembly. US 20030137320 A1, 2004. [36] C. N. Lau, W. Bao, J. Velasco Jr, Mater. Today 2012, 15 (6), 238. [37] V. Varshney, S. S. Patnaik, A. K. Roy, G. Froudakis, B. L. Farmer, ACS nano 2010, 4 (2), 1153. [38] Y. Wang, S. Chen, X. Ruan, Appl. Phys. Lett. 2012, 100 (16), 163101. [39] Y. Wang, B. Qiu, X. Ruan, Appl. Phys. Lett. 2012, 101 (1), 013101. [40] N. Wei, L. Xu, H.-Q. Wang, J.-C. Zheng, Nanotechnology 2011, 22 (10), 105705.

8 www.small-journal.com

[41] G. Zhang, H. Zhang, Nanoscale 2011, 3 (11), 4604. [42] J. Chen, G. Zhang, B. Li, arXiv preprint arXiv:1005.4481 2010. [43] W. Humphrey, A. Dalke, K. Schulten, J. Mol. Graphics Modell. 1996, 14 (1), 33. [44] S. Shenogin, R. Ozisik, Polymer 2005, 46 (12), 4397. [45] D. W. Brenner, O. A. Shenderova, J. A. Harrison, S. J. Stuart, B. Ni, S. B. Sinnott, J. Phys.: Condens. Matter 2002, 14 (4), 783. [46] D. Wei, Y. Song, F. Wang, J. Chem. Phys 2011, 134, 184704. [47] S. J. Plimpton, J. Comput. Phys. 1995, 117 (1), 1.

© 2015 Wiley-VCH Verlag GmbH & Co. KGaA, Weinheim

Received: December 20, 2013 Revised: December 3, 2014 Published online:

small 2015, DOI: 10.1002/smll.201303888